<<

diagrams

0.44 wt% of in Fe microstructure of a of eutectic composition

Primer For Science Teaching Spring 2018 28.6.2018 What is a phase?

A phase may be defined as a homogeneous portion of a system that has uniform physical and chemical characteristics Phase Equilibria • Equilibrium is a thermodynamic terms describes a situation in which the characteristics of the system do not change with time but persist indefinitely; that is, the system is stable • A system is at equilibrium if its free is at a minimum under some specified combination of , , and composition. The Gibbs This rule represents a criterion for the number of phases that will coexist within a system at equilibrium.

Pmax = N + C C – # of components ( that is single phase; has specific ; and has a defined / point)

N – # of variable thermodynamic parameter (Temp, Pressure, Electric & )

Pmax – maximum # of phase(s) Gibbs Phase Rule – example of C = 1 N = 1 (fixed pressure or fixed temperature) P = 2 fixed pressure (1atm)

0 0C 100 0C melting 1 atm. fixed pressure (0.0060373atm=611.73 Pa) Ih vapor

0.01 0C sublimation fixed temperature (0.01 oC)

vapor liquid solid

611.73 Pa 109 Pa The Gibbs Phase Rule (2) This rule represents a criterion for the number of degree of freedom within a system at equilibrium. F = N + C - P F – # of degree of freedom: Temp, Pressure, composition (is the number of variables that can be changed independently without altering the phases that coexist at equilibrium)

Example – Single Composition 1. For single phase (P=1): F = 2 + 1 - 1 = 2 (area) . can play with P and T. 2. For two phases (P=2): F = 2 + 1 – 2 = 1 (line) . each temp determined the pressure 3. For three phases (P=3) : F = 0 (point). no freedom at all. pressure, and temperature are fixed!

Example – Binary Composition (Const Pressure  N=1) 1. In the case of one phase: F = 1 + 2 - 1 = 2. one has two degree of freedom to maintain one phase. i.e. Temp and compositions 2. In the case of two phases: F = 1 + 2 - 2 = 1. Only one degree of freedom. Each

Temp determine the compositions Cα and CL. 3. In the case of three phase: F = 1 + 2 - 3 = 0. one has NO degree of freedom i.e. it’s a single point (eutectic point) Binary phase diagram

Full (Cigar shape diagram) Partially solubility (eutectic diagram) Full Solubility (Cigar shaped diagram) In Cigar shape diagram there are three different regions: 1. Liquid (single phase) 2. Liquid + solid (double phase) 3. Solid (single phase) •- the boundary line between the liquid region and the double phase region. •- the boundary line between the region and the double phase region. For Cigar shape diagram three parameters are available: 1. Phase presents: just locate the Temperature-Composition point and determine the phase(s) 2. Phase composition. 3. Phase amount (in the double phase region) – The

At the point B: •Phase composition •The Ni composition of the liquid

phase is CL •The Ni composition of the solid α

phase is Cα •Phase amount •Amount of the liquid phase is:

•Amount of the Solid phase is: Example - Equilibrium Cooling

A alloy of composition 35 wt% Ni – 65 wt% Cu is slowly cooled from 1300 oC (a)At what temperature does the first solid phase form? • Around 1250 oC (b) What is the composition of this solid phase? • 46 wt% Ni (c) At what temperature does complete solidification of the alloy occur? • Around 1210 oC (d) What is the composition of the last liquid remaining prior to complete solidification? • 24 wt% Ni (e) What is the amount of the solid phase at point c You start to solution of 60 wt% of Cr2O3 from room temperature up to 2200 oC a)What is the melting Temp of pure? Al2O3 and of pure Cr2O3? o A • 2045 C for Al2O3 and 2275 for Cr2O3 b)At which Temp the first liquid appears? • Around 2110 oC-2120 oC c)What is the weight percentage of Cr2O3 in the first liquid phase formed • Around 35% d)At which Temp all of the solution transformed to liquid • Around 2190 oC e)What is the composition of the last solid just before melting

• Around 85% Cr2O3 f)What is the amount of liquid and solid phases at the point A (around 2150 oC)

W  100  44  56% Non-Equilibrium Cooling

For Large cooling rate there is not enough time for ! Partially solubility (eutectic diagram)

Single phase Double phase Three phases In Eutectic shape diagram there are features that are not exist in Cigar shape diagram : • Solvus- the boundary line between the solid solution region and the double phase region solid region. This line together with the solidus line indicate the solubility limit of the solid solution (max component b in α / max component a in b) in each temperature. • Eutectic Line- line where three phases co-exist (α, β, L); below this line (temperature) there is a complete solidification. • Eutectic Point- a point (composition) on the eutectic where the melting and solidification are like in a single component diagram; The melting temperature is the lowest for the Eutectic composition. • Max Solubility Limit- is the max amount of component b in α / max amount of component a in b. The max solubility limit is always at the eutectic temperature. Example - Gibbs phase rule in eutectic diagram

In the double phase regions: N = 1 (the diagram is plotted for fixed pressure, 1 atm) C = 2 P = 2 F = 2 F = N + C -P F = 0

In the single phase regions: N = 1 (the diagram is plotted for fixed pressure, 1 atm) C = 2 F = 1 P = 1 F = N + C -P

At the eutectic line: N = 1 (the diagram is plotted for fixed pressure, 1 atm) By fixing the Temp one determines the C = 2 compositions in the liquid and in the P = 3 solid F = N + C -P i.e. for certain Temp there is a fixed compositions Microstructure obtained with different compositions Primary α eutectic α

lamellae Calculating amounts

Amount of eutectic structure

Amount of primary α

Amount of total α phase

Amount of total β phase (eutectic) You start with 10 kg solution of 10 wt% Sn - 90 wt% Pb at 200 oC a)How many phases do you have? • 1, α phase b)You continue to heat. At which temp will the first liquid appear? What is the wt% of Pb in this first liquid? • Around 280 oC. 78 wt% Pb c)You start to cool your solution. At which temp the first β phase appears? What is the wt% of Pb in this first β phase ? • Around 150 oC. Around 3 wt% Pb d)At 100 oC what is the amount in kg of the α phase? What is the amount of the β phase? 10  5 wt%( b )   5% • Using the lever rule to find the amount of b: 98  5 = 0.5 kg e) What is the wt% Pb of the α and β phase at 100 oC • 95% and 2% respectively Complex Diagrams Complex Diagrams

(bTi)

C

° Temp., Temp.,

%Cu Ti2Cu Cooling Curves

pure component pure component with

Time

full solubility

eutectic DSC- Differential scanning calorimetry How you think the DSC graphs (heat flow Vs temperature, 0.25 o/min cooling to -30oC then heating to 5oC) of pure water and water + 4.76wt% NaCl will look like? 40 water heating

0

Heat Flow (mW)

cooling

-40 -30 -25 -20 -15 -10 -5 0 5 T (oC)

water+4.76wt% NaCl 30 heating 20 10 0 -10 -20

Heat Flow (mW) Heat Flow -30 cooling -40 -50

-30 -25 -20 -15 -10 -5 0 5 T (oC) 40 water heating

0 cooling

Heat Flow (mW)

-40 -30 -25 -20 -15 -10 -5 0 5 T (oC)

water+4.76wt% NaCl 30 heating 20 10 0 -10 cooling -20

Heat Flow (mW) Heat Flow -30 -40 -50

-30 -25 -20 -15 -10 -5 0 5 T (oC)